**E**

**dición**

**digit**

**al**

**S. Gómez-Jimenez1 _{, A.M. Becerra-Ferreiro}1_{, E. Jareño-Betancourt}1_{, }**

**R. Castañeda-Miranda1 _{, J. Vázquez-Penagos}2_{, S. Aranda-Espinoza}3**

1_{Universidad Autónoma de Zacatecas, Unidad Académica de Ingeniería}

Av. López Velarde 801, Zacatecas, Zac., México.

2_{Elastomer Solutions México S de R. L. de C. V.}

Circuito Fresnillo Poniente 21 s/n, Parque industrial Fresnillo, Zacatecas, México.

3_{Universidad Autónoma de San Luis Potosí, Instituto de Física}

Av. Manuel Nava 6, Zona Universitaria San Luis Potosí, 78290 México.

**Abstract**

The precise control of curing reaction parameters allows a better crosslinking polymer. Modeling and optimization of this process require a correct kinetic of curing model. The kinetics of the crosslinking reaction is studied for the ethylene propylene diene monomer (EPDM) synthetic elastomer by movile die rheometer (MDR). The kinetic parameters of reaction were calculated from Kamal-Ryan, Sestak-Berggren, and the Isayev-Deng methods at different temperatures. An Arrhenius-type function for the order of reaction n is introduced to improve the adjusting. A comparative study of Sestak-Berggren and Isayev-Deng models was made to validate and determine which model best describes the behavior of vulcanization. The best approximation was obtained with the model Isayev-Deng. Finally, taking the model with the best fit, a graphical and analytical description of the cure kinetics was developed. The order of reaction is predicted to better establishment of processing time. It was noted that for EPDM at higher temperatures, the increase of the rate of reaction occurs in short period of time, which could cause premature curing if the supply system is inadequate.

**Resumen**

El control preciso de los parámetros de reacción de curado permite un mejor reticulado del polímero. El modelado y la op-timización de este proceso requiere una adecuada descripción de la cinética de curado. En el presente trabajo se estudia la cinética de la reacción de curado para el elastomero sintético monómero propileno-dieno (EPDM) por medio de un reóme-tro de cámara móvil (MDR). Los parámereóme-tros cinéticos de la reacción se calcularon a partir de los métodos de Kamal-Ryan, Sestak-Berggren e Isayev-Deng a diferentes temperaturas. Para mejorar el ajuste se introdujo una función tipo Arrhenius para el orden de reacción n. Se hizo un estudio comparativo entre los modelos de Sestak-Berggren e Isayev-Deng para vali-dar y determinar cuál modelo describe mejor el comportamiento de vulcanizado del polímero ensayado. Se predice el orden de reacción para una mejor descripción del tiempo de procesamiento. Se observó que, para el EPDM a las temperaturas más altas ensayadas, el incremento de la fracción de curado ocurre en periodos de tiempo cortos, lo que podría ocasionar curado prematuro si el sistema de inyección es inadecuado.

**Vol. 6 No. 4 (2019) 123 - 132**

**Phenomenological effect of temperature on the order **

**n**

** of the**

**reaction of the curing kinetics in an EPDM polymer**

**Efecto fenomenológico de la temperatura en el orden n de reacción de la cinética de **

**curado en un polímero EPDM**

Fecha de recepción: 04-10-2018 Fecha de aceptación: 14-01-2019

**Introduction **

Vulcanization is one of the essential processes in the rubber industry, involves an enormous amount of energy to convert a material without form into an elastic finished product [1]. Elastomers consist of independent high molecular weight molecules when they are in the monomer or non-vulcani-zed states. The cross-links between these molecules show nonlinear viscoelastic behavior allowing the flow and pro-cessing by injection. During the injection, a chemical reac-tion of vulcanizareac-tion (or curing) takes place. The vulcani-zing process presents three stages: induction, curing, and post-curing. In the induction stage, reactions of the accele-rators take place, but crosslinks do not occur in the polymer matrix. It has great practical importance since it determines the time when the vulcanization should start and then avoid

premature vulcanization. The curing stage begins with the formation of crosslinks at a curing rate that depends on the temperature and the composition of the rubber. Up to approximately 90% of vulcanization take place, and it is measured with the proportional increase in elasticity. If curing is continued post-curing occurs (final stage); this can cause a hardening or soften of the product which are usually undesirable effects [2].

The curing rate increases with temperature and therefore a finite time for filling the mold is needed [3, 4]. The final pro -perties of the formed polymer depend largely on reactions that occur during vulcanization, so it is necessary to study the curing kinetics of the compound to determine the time and degree of curing [5, 6].

**Palabras clave: **

Cinética de curado, Reología de polímeros, Parámetros ciné-ticos, Modelos fenomenológicos

**Keywords:**

Curing Kinetics, Polymer Rheology, Kinetic Parameters, Phenomenological Models

**E**

**dición**

**digit**

**al**

The rubber curing is an exothermic process of high comple-xity in which several reactions coincide [7, 8]. The vulca-nization mechanism and the rate of reaction depend on the structure of the rubber, the concentration of activators and accelerators as well as the diffusivity, and thermodynamics of each reaction [9].

The reaction rate means how quickly the concentration of a reactant or a product changes over time. Several mathemati-cal models used to describe the semi-solid chemimathemati-cal kinetics present inconsistencies among them [10]. This may be due to the difficulty in distinguishing between a reaction regi-men controlled by the mass, that is thermo-mechanical, or a reaction regimen controlled by diffusion [11].

On the other hand, the kinetics associated with a chemical process is not correctly characterized by the so-called ki-netic triplet. That is activation energy, pre-exponential fac-tor and kinetic model which are represented either by a diffe-rential function f(a) or by an integral function g(a). Where a is the cure rate. Knowing the f(a) or g(a) functions, the characterization of the chemical process could be solved. In the majority of cases, these functions are unknown or are too complicated. In order to have a better description of the process a simplify models are necessary to describe the system behavior approximately. Such phenomenological or empirical models tend to ignore de chemical details of the system [11].

It is common to rename the molar concentration of chemical reactions for the so-called degree of cure, conversion or cure rate α, which is normalized by any other physical time-de-pendent property that represents the system. In this paper, the viscosity of Mooney (rheometer torque) was used since it can be normalized as the rate of conversion α [12].

Due to the complexity of the cure kinetics, models of order n are used to describe the reaction paths since they are se-quential and parallel. These models allow a better approxi-mation to describe the behavior of the vulcanization rate in terms of an autocatalytic reaction. The most widespread and best fit include Kamal-Ryan, Sestak-Berggren, and Isa-yev-Deng models, from which the curing rate can be mode-led by determining the kinetic parameters involved such as the order of reaction and the rate constants. Most of authors considered the order of reaction as the average of the values obtained at different temperatures [13, 14]. Recent publica-tions present variety of polynomial models to describe order of reaction as a temperature variation dependent [15, 16].

This research consisted in adjusting the parameters of the
Kamal-Ryan expression in the curing kinetics of the EPDM
rubber by proposing an Arrenius-type function for the
or-der of reaction *n* (temperature variation dependent). Then
a comparative study of the models of Sestak-Berggren and
Isayev-Deng, for describing the cure kinetics using the
proposed expression, was carried out in order to

ascer-tain which of these models better describes the behavior
of EPDM polymer. By taking the model with the best fit,
a graphical and analytical description of cure kinetics was
developed in a three-dimensional field a(*T*, *t*).

**Materials and Methods**

**Materials**

Synthetic elastomer EPDM (ethylene propylene diene
mo-nomer M-class was used, according to the standard ASTM
D1418 – 17. Standard Practice for Rubber and Rubber
Latti-ces-Nomenclature) with Sulphur as a vulcanizing agent and
integrated lubricant (black carbon). Tested under standards
GMW 14744 type B with reference to standards SAE J200,
ASTM D2000, GMW 3232 compatible with standard
FM-VSS302, GMW 3059 for substances restricted and
repor-table. ISO 48 (55 +/- 5) hardness IRHD, resistance to
tem-perature 24 h (90 +/-3) °C with no changes in function and
appearance. The test specimen was prepared at 20°C
tempe-rature with 5 *cm*3_{ (25 }_{mm}_{ × 25 }_{mm}_{ × 8 }_{mm}_{) sample volume.}

**Method**

Trials were conducted in an Alpha Technologies Moving Die Rheometer (MDR 2000), property of Elastomer Solu-tions México S. de R. L. de C. V, according to the standard ASTM D2084 – 01. This type of cure meter measures the torque produced by an angular strain of constant amplitude in a cavity that is completely closed and sealed (see Figure 1a). The die cavity is formed by two dies (Figure 1b). In the measuring position, the two dies are fixed a specified distan-ce apart so that the cavity is closed and sealed. A pneumatic cylinder closes the dies and holds them closed during the test with a force of not less than 8.0 kN (1820 lbf).

**Figure 1**, Sealer torsion shear rotorless curemeter, ASTM D 5289 – 12:
(a) Measuring principle, (b) Reaction dies.

The die oscillating system consists of a rigid eccentric drive, which imparts a torsional oscillating movement to one of the dies, in the plane of the cavity. This action produces a sinusoidal alternating torsional strain in the test piece and a sinusoidal shear force or torque, which depends on the sti-ffness (shear modulus) of the rubber compound. The

**E**

**dición**

**digit**

**al**

tude of the oscillating torque is continuously recorded as a function of time and torque against time graphs are obtained (Figure 2).

**Figure 2**, Standard graph time vs. torque, where ML and MH, represent

the minimum and maximum torques; ti is the induction time, ts2 is the

time to incipient cure (scorch time), and t_{90} is the time to reach 90% of

final crosslinking.

The trial was conducted with amplitude of oscillation from 0 to 5 degrees and a frequency of 1.66 Hz, according to the standard ISO 6502-1999 and ASTM D5289 - 12(Standard Test Method for rubber property-vulcanization using os-cillating disk cure meter) with isothermal permanence of samples at different temperatures ranges, 155 to 205°C with increments of 10°C each.

In order to convert the rheometry test results into time varia-tions of the state of cure, the following Equation was used.

α =

### (

−### )

−### (

*MM MM*

### )

*t* *L*

*H* *L* _{ }

(1)

where a is the cure rate, *M _{t}*,

*M*, and

_{L}*M*is the instant, minimum and maximum torques, during the reaction res-pectively.

_{H}**Models for describing the cure kinetics**

Generally, the cure kinetics is expressed with the following differential equation

*d*

*dtr* *K T f*

α _{α}

=_{}

### ( )

_{}

### ( )

(2)

Where *K*(*T*) is the kinetic constant and *f*(a) is a function of
the cure degree; *t _{r}* is the reaction time, that corresponds to
the total process time t minus induction time

*t*.

_{i}*tr*= −*t ti* _{ (3)}

Claxton-Liska isothermal model defines the induction time t_i with an Arrhenius-type temperature dependence equa-tion [17, 18]:

*t t ei* = 0 *T T*0/ _{ (4)}

Kamal-Ryan model [19] was initially developed to describe
the gradual reaction mechanism in rubber materials using
two parameters for the order of reaction (*m*, *p*) and two rate
constants (*k*_{1}, *k*_{2}) as shown in equation (5). In this model, the
total order of reaction n is considered as (*m*+*p*).

*d*

*dtr* *k k*

*m* *p*

α _{α} _{α}

=

### (

1+ 2### )

### (

1−### )

(5)

with (0 ≤ *m *≤ 1, *p *≥ 1) [2], while Sestak-Berggren model
presents just one kinetic constant

*K T*

### ( )

*k T*

=

### ( )

_{ }(6)

and the degree of curing function as the following expres-sion

*f* *m* *p*

α α α

### ( )

=### (

1−### )

(7)

the reaction rate can be written as

*d*
*dtr* *k T*

*m* *p*

α _{=}

_{( )}

_{α}

_{(}

_{−}

_{α}

_{)}

1
(8)

*k* is the temperature-dependent rate constant, α is experi
-mentally calculated using equation 1, *k* follows the
Arrhe-nius law:

*k T* *k e*

*E*
*RT*

### ( )

= −
_{}

0 _{ }(9)

where *k*_{0} is the pre-exponential factor (temperature
inde-pendent), *E* is the activation energy, *R* is the universal gas
constant and *T* is the temperature.

From equation (2) and (6), time curing is expressed as a function of α as:

*k T dt* *d*

*t*

*m* *p*

*r*

### ( )

=

−

### (

### )

### ∫

0### ∫

01 1

α α α

α

(10)

Solving the last equation results in

*t*

*k T* *m* *F* *m p* *m*

*r*

*m*

=

_{( )}

−
### (

### )

### (

− −### )

−

α1 _{α}

1 1 , ;2 ; _{ }(11)

**E**

**dición**

**digit**

**al**

where *F* is a hypergeometric function which can be defined
as follows:

*F* *m p* *m* *m p*

*m*

*m* *m p p*

*m*

1 2 1 1

1 2

1 2 1

2 2 3

− −

### (

### )

= +### (

−### )

−### (

### )

+ +### (

−### )

### (

−### )

### (

+### )

−### (

### )

− , ; ; ! ! α α*m*

*m*

*m* *m* *m p p* *p*

*m* *m* *m*

### (

### )

+ +### (

−### )

### (

−### )

### (

−### )

### (

+### )

### (

+### )

−### (

### )

### (

−### )

### (

−### )

+ α α 2 31 2 3 1 2

3 2! 3 4 ... _{ }

(12)

Alternatively, equation (10) can be expanded using Taylor series before being integrated to obtain the same result.

On the other hand, the empirical model proposed by Isayev - Deng to determine the parameters of the cure kinetics [7, 20-22] is expressed by the following equations:

*K T*

### ( )

=*k T*

### ( )

*n*

1

(13)

*f*

_{( )}

_{α}

_{=}

*n*

_{α}

*n*−

_{1}/

*n*

_{(}

_{1}

_{−}

_{α}

_{)}

*n*+1/

*n*

(14)

Substituting equations (13) and equation (14) in equation (2), we can obtain the following expression

*d*
*dtr* *nk*

*n* *n* *n* *n* *n*

α _{=} 1/_{α}(−1)/

_{(}

_{1}

_{−}

_{α}

_{)}

( +1)/
(15)

Considering the empirical model proposed by
Kamal-Sou-rour [23]:
α =
+
*kt*
*ktr*
*n*
*rn*

1 _{ }(16)

and substituting equations (16) in equation (15), the reduced model is obtained

*d*
*dt*
*nkt*
*kt*
*r*
*rn*
*rn*
α
=
+

### (

### )

−1 2 1 (17)where *n*≥1.

Equation (16) describes a reaction that slows down quickly
as conversion progresses, such that limα(*t*)=1 due to the
de-pletion of reagents so 0 < α <1.

Expressing the curing time as a function of

### α

, from equation (16) results:*t*

*k*

*r*

*n*= −

### (

### )

α α 1 1 (18)Using logarithms we obtain:

ln *t* ln

*nLn* *n* *k*

*r*

### ( )

= − + 1 1 1 1 αα _{ } _{ }(19)

From expression (19), plotting ln(*t _{r }*) vs ln[α⁄(1-α)], for any
given test temperature, results in parallel lines with slope
1/

*n*[22].

On the other hand, to obtain the reaction rate using the re-sults obtained with the equation (1), the method of finite di-fferences is applied as shown in equation (20):

*d*

*dtr* *t*

*j* *j*

*r*

α α α

= − −1

∆ _{ }(20)

The literature cites a variety of differential models to des-cribe the curing kinetics through a phenomenological approach.

In this work, the rheometric characterization of EPDM
polymer is experimentally obtained, whereas the curing
rate adjustment is made using the empirical models of
Ses-teake-Berggen (with parameters [*k*, *m*, *p*)]) and Isayev-Deng
(with parameters [*k*, *n*]) in order to ascertain which model
best describes the behavior of the polymer.

**Results and Discussion**

The curing kinetics of EPDM polymer obtained by
non-li-near adjustments from six different isothermal tests
ca-rried out in the MDR 2000 appliance. Kinetic parameters
from non-linear fits are tested with the Kamal-Sourour
adjustment. The analysis of variation of each parameter
as a function of temperature was developed. Kinetic
mo-dels of Sestake-Berggen (*k*, *m*, *p*) and Isayev–Deng (*k*, *n*)
is used to obtain the adjusted-parameters set from each
model.

**Rheological tests **

Figure 3 shows the graphs obtained from tests carried out at various temperatures in the MDR 2000 instrument. This shows a non-reversible behavior because the torque re-mains constant after reaching the maximum value. Results also shown that induction times became shorter as the test temperature was increased since it is a characteristic be-havior in the vulcanization of sulfur-containing polymers [24].

Table 1 shows results obtained from a test carried out in the Alpha Technologies MDR 2000 (Moving Die Rheometer) for each of the parameters. Also, induction time (when mi-nimum torque occurs) is included.

(t→∞)

**E**

**dición**

**digit**

**al**

**a)**

**b)**

**Figure 3**, (a) Isotermal rheometry tests; (b) Induction times

**Table 1**, EPDM cure-characteristics obtained at different temperatures
T

(°*C*)

ML
*dN*-*m*

MH
*dN-m*

*ti*

*min*

*ts*2

*min*

*t*90

*min*

155 1.00 6.38 0.29 1.94 12.10

165 0.95 6.52 0.22 1.21 10.98

175 0.94 7.58 0.20 0.90 7.68

185 0.93 7.61 0.18 0.56 4.83

195 0.89 7.82 0.15 0.42 2.90

205 0.87 8.20 0.13 0.34 1.52

Figure 4 represents the degree of curing variation depending on reaction time,

### α

is obtained from rheometric tests using equation (1). This graph shows the non-linear dependence of the degree of curing related to time and temperature. Allows us to obtain kinetic parameters from non-linear fits for each temperature being tested. Also, it was observed that during the first four minutes the polymer reaches approximately 60 to 90 percent of curing.**Figure 4**, Standardized curing-degree graphics using equation (1)

The adjustment of these results with Kamal-Sourer expres-sion (equation (16) is represented in Figure 5.

**Figure 5**, Curves adjustment using equation (16), based on the MDR tests

The appropriate fitting data results in a correlation R2_{ of }

0.99 and higher for all cases, see Table 2. The
correspon-ding curing-kinetic parameters *k*, *n* and *t _{i}* are also reported
in this table.

**Table 2**, Adjusted values of *k*, *n *and *ti* at different temperatures using the

expression (15)

T

(°C) *k* *n*

*t _{i}*

*min* *R*

2

155 0.08 1.81 0.29 0.9992

165 0.27 1.59 0.22 0.9997

175 0.62 1.53 0.2 0.9993

185 1.05 1.43 0.18 0.9991

195 1.89 1.25 0.15 0.9995

205 3.71 1.19 0.14 0.9991

**Variation of curing parameters with temperature**
Once determined the isothermal behavior of the curing-degree
with each tested temperatures, the analysis of variation of each
parameter as a function of temperature was developed.
In Figure 6, it is observed that the constant of reaction-rate

*k* increases rapidly as the temperature of the test increases.
This behavior agrees with the Arrhenius model (equation
(9)). In this case, the adjustment of *k*(*T*) using Arrhenius
co-rrelates with *R*2_{ = 0.9951.}

**Figure 6**, Adjustment of k using equation (9)

**E**

**dición**

**digit**

**al**

For induction-time *t _{i}* (

*T*), the adjustment was carried out with the Claxton-Liska model equation (4) obtaining R2

_{ = }

0.9864. Figure 7 shows the corresponding graph.

**Figure 7**, Fitting of t_i using Table 2 data and equation (4)

When experimental data using equation (19) it is expected
to get straight parallel lines with the 1⁄n slope. However, it
was found that the slopes are different for each temperature
which suggests that, for the tested material, the order of
re-action n also depends on temperature. Figure 8 also shows
that the order of reaction * n* varies non-linearly as increases
sampling isothermal-temperature.

**Figure 8**, Behavior of *ln*(*n*) vs 1/*T*

So, to describe how the order of reaction *n* varies, an
Arr-henius-type expression was proposes based on the trend
shown in Table 2 and Figure 8. The expression is indicated
by equation (21).

*n n e*

*T*
*aT*
=

0

0

(21)

where a is the material´s constant obtained by non-linear
re-gression of experimental results, see Table 3. It can be
infe-rred, from the curve shape of Figure 9, that *a* > 1.

In Figure 9, the fitted experimental results using the
pro-posed expression are plotted. The reliability factor is high
enough R2_{ = 0.9896, that is an error of just 1.04%. }

**Figure 9**, Adjustment of * n* based on the Table 2 data and equation (21)

Table 3 lists the values of the constants used in the
calcu-lation of the parameters *k*(*T*), *t _{i}* (

*T*) and

*n*(

*T*) for the Ka-mal-Sourour model.

**Table 3**, Constants for calculation of Kamal-Sourour model

*T*0 (*K*)

*k*0

(min-1_{)} *n*0 *a*

*t*0

(*min*)

*E*
*R*

*mol K*
*Kg*

_{}

3,165 3.99e+08 3.6499e-2 2.16 1.43e-4 8,822

**Comparison between Isayev-Deng and **
**Ses-ták-Bergger models for the curing rate**

In order to validate the proposed expression for the reaction
order, first the variations of the parameters *k*(*T*), *t _{i}* (

*T*) y

*n*(

*T*) were substituted in the kinetic models of Sesták-Berggen (

*k*,

*m*,

*p*), equation (8), and Isayev–Deng (

*k*,

*n*), equation (17). Table 4 shows the adjusted-parameters set from each model.

**Table 4**, Parameters obtained using non-linear adjustments of kinetic models

*T *(℃) *Isayev-Deng* *Sesták-Berggen*
*k*(*T*) *n*(*T*) *k*(*T*) *m* *p* *n*
155 0.0856 1.805 0.4771 0.4669 1.5747 2.04
165 0.2444 1.622 0.7454 0.4081 1.6676 2.07
175 0.5589 1.504 1.2463 0.4074 1.7111 2.11

185 1.0506 1.324 1.7394 0.3866 1.7831 2.16 195 1.9547 1.278 2.9667 0.4440 1.7974 2.24 205 3.6677 1.202 4.8921 0.3073 2.0055 2.31

Subsequently, the curing rate was calculated from the ex-perimental results using the equation (20) to make the ad-justment with each of the above models. This also allowed knowing which of two models best describes the curing ki-netics of EPDM polymer.

The solution obtained with equation (17) and equation (8) against the equation (20) at all considered operating tempe-ratures, are contrasted in Figure 10. Corresponding reliabi-lity factors are shown in Table 5.

In both cases, the reliability factor R2 is high enough to con-sider that the expression proposed for the temperature-de-pendent order of reaction is entirely accurate for the tested material. On the other hand, although both models adequa-tely describe the phenomenon, the best fit is obtained with the Isayev-Deng model.

**.**

**E**

**dición**

**digit**

**al**

**Table 5**, Correlation coefficients between equation (20) and equations

(17) and (8)

*T*(℃) *Isayev-Deng*
*R*2

*Sesták-Berggen*
*R*2

155 0.9998 0.9981

165 0.9998 0.9982

175 0.9998 0.9986

185 0.9998 0.9888

195 0.9998 0.9879

205 0.9998 0.9874

In the case of Sesteake model, after the curing rate reaches its maximum and begins to decline, the gap between experimen-tal results and this model increases slightly. This separation respect to the Isayev model is minimal (see graphs of Figure 10). Another notable advantage of Isayev-Deng kinetic model is that it uses only two parameters (k,n), as the Sesták-Berg-gen model requires three (k,m,p); this advantage could make more accessible programming the rate of curing.

In Figures 11 and 12 the curing-kinetics behavior as tem-perature increases is described using the expression with the best fit and fewer parameters. Note that, as temperature takes higher values, the maximum reaction rate takes place in less time and becomes higher (Figure 11); this occurs in the range of curing fraction α less than 0.25 (Figure 12).

The resulting values for the maximum curing rate obtained from the Isayev-Deng model are shown in Table 6. It is also shown the drastic reduction of α at peak curing rate. These results indicate that the vulcanized can be defective if the variables of time and temperature are not adequately con-trolled.

a) b)

c) d)

e) f)

**Figure 10**, Plots of cure kinetics at different temperatures from standardized experimental data and the adjusted models of Sesták – Berggen and Isayev -
Deng: a) *EPDM to* 155º, b) *EPDM* to 165º, c) *EPDM* to 175º, d) *EPDM* to 185º, e) *EPDM* to 195º and f)* EPDM* to 205º

**E**

**dición**

**digit**

**al**

**Figure 11**, Reaction rate vs time

**Figure 12**, curing rate against the degree of curing

**Table 6**, Maximum curing rate*d _{dt}*a vs

*and*

**t***to different temperatures*

**α***T*
(°C)

*t _{r}*

(min) **α**

*d*
*dt*

a
(min-1_{)}

155 1.9696 0.2233 0.1591 165 0.9017 0.1857 0.2628 175 0.4967 0.1740 0.4438 185 0.2899 0.1515 0.6362 195 0.1061 0.1016 1.0792 205 0.0412 0.0791 2.0609

Figure 13 illustrates the three-dimensional behavior of the
transformation ratio as a function of time and the reaction
temperature *α* (*T*, *t _{r }*). This graph provides the theoretical set
of values that describe in a wide range the fraction of curing
for the EPDM material tested.

For future, the kinetic model could be used in the simulation of the EPDM injection process since the reaction rate is inti-mately related to the heat generation [25], see equation (22).

Q = Q_{∞}*d*

*dt*

α

(22)

**Figure 13**, Surface graphics α(T, tr)

**Conclusions**

It was possible to obtain, through adjustments of nonlinear regression, the kinetic parameters of kamal-Sourour expres-sion for the EPDM material.

From the experimental results, it was found that the order of
reaction is a temperature dependent parameter and it obeys
to an Arrhenius-type exponential function. The fitted
ex-perimental results using the proposed expression determine
a reliability factor good enough, R2_{ = 0.9896. That }

corres-ponds to a relative error of just 1.04%.

Each of the parameters involved in Kamal-Sourour model
for the degree of curing could be expressed in function
of the temperature, allowing to extend the behavior to a
three-dimensional model *α*(*T*, *t*).

The adjusted model of Isayev–Deng was contrasted with the one of Sesták – Berggen. It was found that Isayev-Deng model best describes the kinetics of reaction in the tested isothermal temperature range.

As temperatures increase, the maximum reaction rate takes place in less time than the normal and rises high values for the curing processes. This could cause premature curing if the design of the rubber feeding system is not adequate.

Finally we can conclude that since Deng-Isayev model uses the minimum of parameters to describe the kinetics of cu-ring, it can be used more efficiently to EPDM polymer injec-tion-process simulation.

**Acknowledgments**

We want to thanks Elastomer Solutions México S. de R. L. de C. V., Condensed Soft Matter Network, and CONACyT for support provided to this research.

**E**

**dición**

**digit**

**al**

**References**

[1] Pantani, R., *Validation of a model to predict birefrin*

*-gence in injection molding*. European Polymer Journal,
2005. 41(7): p. 1484-1492.

[2] López-Manchado, M.A., et al., *Vulcanization kinetics *

*of natural rubber–organoclay nanocomposites*.
Jour-nal of Applied Polymer Science, 2003. 89(1): p. 1-15.

[3] Guerrier, P., G. Tosello, and J.H. Hattel, *Flow visualiza*

*-tion and simula-tion of the filling process during injec*

*-tion molding*. CIRP Journal of Manufacturing Science
and Technology, 2017. 16(Supplement C): p. 12-20.

[4] Restrepo-Zapata, N.C., et al., *Chemorheological ti*

*-me-temperature-transformation-viscosity * *diagram: *

*Foamed EPDM rubber compound*. Journal of Applied

Polymer Science, 2016. 133(38): p. n/a-n/a.

[5] Kader, M.A. and C. Nah, *Influence of clay on the vul*

*-canization kinetics of fluoroelastomer nanocomposites*.
Polymer, 2004. 45(7): p. 2237-2247.

[6] Milani, G. and F. Milani, *Kinetic finite element model to *

*optimize sulfur vulcanization: Application to extruded *
*epdm weather-strips*. Polymer Engineering & Science,
2013. 53(2): p. 353-369.

[7] Hong, I.-K. and S. Lee, *Cure kinetics and modeling the *

*reaction of silicone rubber*. Journal of Industrial and
Engineering Chemistry, 2013. 19(1): p. 42-47.

[8] Likozar, B. and M. Krajnc, *A study of heat transfer *

*during molding of elastomers*. Chemical Engineering
Science, 2008. 63(12): p. 3181-3192.

[9] Crié, A., et al., *Rheological behavior of uncured styre*

*-ne-butadiene rubber at low temperatures, pure and fi*

*-lled with carbon black*. Polymer Engineering &
Scien-ce, 2015. 55(9): p. 2156-2162.

[10] Koga, N., et al., *Data Treatment in Non-isothermal Ki*

*-netics and Diagnostic Limits of Phenomenological Mo*
*-dels*. Netsu Sokutei, 1993. 20(4): p. 210-223.

[11] Sun, X. and A.I. Isayev, *Cure Kinetics Study of Unfilled *
*and Carbon Black Filled Synthetic Isoprene Rubber.*

Rubber Chemistry and Technology, 2009. 82(2): p. 149-169.

[12] Šesták, J. and J. Kratochvíl, *Rational approach to ther*

*-modynamic rrocesses and constitutive equations in iso*

*-thermal and non-iso-thermal kinetics*. Journal of
Ther-mal Analysis and Calorimetry, 1973. 5(2-3): p. 193-201.

[13] Huang, X. and B. Patham, *Experimental characteriza*

*-tion of a curing thermoset epoxy-anhydride system—*
*Isothermal and nonisothermal cure kinetics*. Journal of
Applied Polymer Science, 2013. 127(3): p. 1959-1966.

[14] Janković, B., *The kinetic analysis of isothermal curing *
*reaction of an unsaturated polyester resin: Estimation *
*of the density distribution function of the apparent ac*

*-tivation energy*. Chemical Engineering Journal, 2010.
162(1): p. 331-340.

[15] Erfanian, M.-R., M. Anbarsooz, and M. Moghiman, *A *

*three dimensional simulation of a rubber curing pro*

*-cess considering variable order of reaction*. Applied
Mathematical Modelling, 2016. 40(19): p. 8592-8604.

[16] Ghoreishy, M.H.R., M. Rafei, and G. Naderi, *OPTIMI*

*-ZATION OF THE VULCANI-ZATION PROCESS OF A *
*THICK RUBBER ARTICLE USING AN ADVANCED *

*COMPUTER SIMULATION TECHNIQUE*. Rubber

Chemistry and Technology, 2012. 85(4): p. 576-589.

[17] Arrillaga, A., et al., *Techniques used for determining *

*cure kinetics of rubber compounds*. European Polymer
Journal, 2007. 43(11): p. 4783-4799.

[18] Khang, T. and Z. Ariff, *Vulcanization kinetics study of *

*natural rubber compounds having different formula*
*-tion variables*. Journal of Thermal Analysis &
Calori-metry, 2012. 109(3): p. 1545-1553.

[19] Keenan, M.R., *Autocatalytic cure kinetics from DSC *

*measurements: Zero initial cure rate*. Journal of
Applied Polymer Science, 1987. 33(5): p. 1725-1734.

[20] Lopez, L.M., et al., *Modeling the vulcanization reac*

*-tion of silicone rubber*. Polymer Engineering &
Scien-ce, 2007. 47(5): p. 675-683.

[21] Rafei, M., M.H.R. Ghoreishy, and G. Naderi,

*Develop-ment of an advanced computer simulation technique for *
*the modeling of rubber curing process*. Computational
Materials Science, 2009. 47(2): p. 539-547.

[22] Yeoh, O.H., *MATHEMATICAL MODELING OF VUL*

*-CANIZATION CHARACTERISTICS*. Rubber

Chemis-try and Technology, 2012. 85(3): p. 482-492.

[23] Kamal, M.R. and S. Sourour, *Kinetics and thermal cha*

*-racterization of thermoset cure*. Polymer Engineering
& Science, 1973. 13(1): p. 59-64.

**E**

**dición**

**digit**

**al**

[24] Albano, C., et al., *Characterization of NBR/bentonite *

*composites: vulcanization kinetics and rheometric and *
*mechanical properties*. Polymer Bulletin, 2011. 67(4):
p. 653-667.

[25] Lee, W.I., A.C. Loos, and G.S. Springer, *Heat of Reac*

*-tion, Degree of Cure, and Viscosity of Hercules 3501-6 *

*Resin*. Journal of Composite Materials, 1982. 16(6): p.
510-520.